Sensors and Achcators A, 43 (1994) 22X29 223
Low-temperature silicon wafer-to-wafer bonding using gold at
Laboratory Electronic Instrumentation, Department of Elecaical
for Engineering, De& Universityof Techno&, Mekehveg 4,
2628 CD De&t (Netherlands)
Centerfor Integrated Sensors and Circuits, Solid-state Electronics Lubomtory, Department of Electrical Engineering and Computer
Ann A&or, MI 48109-2122 (USA)
Science, Uniwsiry of Michigan,
Micromechanical smart sensor and actuator systems of high complexity bemme commercially viable when realized
as a multi-wafer device in which the mechanical functions are distributed over different wafers and one of the
wafers is dedicated to contain the readout circuits. The individually-processed wafers can be assembled using
wafer-to-wafer bonding and can be combined to one single functional electro-mechanical unit using through-
wafer interconnect, provided that the processes invoked comply with the constraints imposed by the proper
operation of the active electrical and micromechanical subsystems. This implies low-temperature wafer-to-wafer
bonding and through-wafer interconnect. Au/Si eutectic bonding has been investigated as it can conveniently be
combined with bulk-micromachined through-wafer interconnect. The temperature control in eutectic bonding has
been shown to be critical.
1. 1ntruductin so that the batch fabrication advantage of the silicon
technology is maintained. This approach, however,
makes low-temperature wafer-to-wafer bonding and
Several practical micromachming techniques in silicon
through-wafer interconnect mandatory.
have emerged from recent research. However, the com-
Two techniques are widely employed for single-wafer
plexity of the micromechanical systems that would po-
micromachining; surface micromachining and bulk mi-
tentially benefit from these developments often exceeds
cromachining. Surface micromachining is based on the
the performance limits of these technologies when
deposition of a sacrificial layer on a silicon substrate,
applied to a single wafer. Silicon wafer-to-wafer bonding
offers the designer of such a system an extra degree the patterning of this layer and the subsequent de-
of flexibility to trade-off single-wafer concentrated com- position of a structural layer. Microstructures remain
plexity for multi-wafer solutions. Wafer-to-wafer bond- in the patterned structural layer after the selective
ing has been used in applications such as power devices removal of the sacrificial layer. In conventional surface
[l], SOI [2-71 and has been particularly successfnl in micromachining with PSG as the sacrificial material,
integrated silicon sensors [&X-11]. the lateral dimensions of fabricated microstructures are
The main advantage of wafer-to-wafer bonding in two orders of magnitude larger than the vertical ma-
the latter application is that it enables the separate chining capability. The lateral dimensions are deter-
fabrication of the sensor wafer and the wafer in which mined by the die size, whereas the non-planarity is
the active readout electronics is integrated, until the limited by the maximum width of the sacrificial layer
very last processing step. The sensor wafer can, there- (about 2-5 pm). Surface micromachining is, therefore,
fore, be designed for maximum performance of the sometimes loosely referred to as a 2; dimensional
sensing element, without jeopardizing the performance sculpturing technique. Bulk micromachining allows the
of integrated active devices; the compatibility is not almost unrestricted sculpturing of a silicon wafer over
impaired. Moreover, the separation also allows for the all three dimensions. Anisotropic etching (usually along
use of different specialized foundries for processing of the (111) planes) or plasma etching enables the fab-
the sensor wafer and the readout wafer. Assembly can rication of wafer-thick cavities or trenches. High-boron-
take place afterwards using relatively simple equipment, doped layers or pn junctions are conventionally em-
Elsevier Science S.A.
ployed to realize an automatic etch stop in order to assumed to take place according to a sequence of
obtain thin membranes, beams and cantilevers. bonding-bridge replacements. Weak OH bridges are
As bulk micromachining is a low-temperature pro- formed at mechanical contact at room temperature.
cessing step, it is compatible with the fabrication of The only voids that are observed in an IR transmission
integrated silicon smart sensors, in which the readout image are due to trapped particles (extrinsic voids) and
electronics are integrated on the chip. However, the the fracture strength remains below 1 MPa. Initial
integrity of the chip is seriously impaired by the (almost) bonding takes place very rapidly and starts at the edge
through-wafer etching of the chip, which results in a where the two wafers make first contact and propagates
reduced yield. This wafer integrity is fully preserved over the wafer surface within a few seconds. Some
in surface micromachining and the low-temperature authors introduce the term ‘bonding wave’ to describe
(LP)CVD techniques, that are used for the deposition the course of the bonding.
of sacrificial and structural layers, ensure compatibility Subsequently, the temperature is increased. Beyond
with integrated readout electronics. The main disad- 200 “C the fracture strength increases and intrinsic void
vantages of the surface micromachining are the limited formation becomes visible. These voids are additional
design flexibility in the vertical direction and the high- to the extrinsic voids. At this stage the hydrogen bond
temperature stress anneal in the structural layer. between OH groups is assumed to be replaced by the
Wafer-to-wafer bonding has the potential to overcome oxygen bridge, whereby water is formed. The pressure
many of these problems. Individual wafers can be of the trapped vapour is assumed to be responsible
subjected to relatively simple bulk and/or surface mi- for the intrinsic void formation. A further increase in
cromachining steps and can subsequently be combined temperature results in dissociation of the water. The
to realize a complex micromechanical function. The fracture strength increases and saturates at about 5
electronic circuits can, in principle, be integrated in MPa, whereas the intrinsic void density decreases. These
any of the wafers, which further improves the design observations are in agreement with the model, as ad-
flexibility. As dicing and packaging take place after ditional oxygen atoms become available to provide
bonding, the micromechanical devices can be designed additional bonds and the hydrogen diffuses through
to be less prone to breaking during fabrication that the silicon lattice. As the vapour dissociates, the voids
would otherwise result from the reduced integrity of dissolve. An alternative theory is based on the lack of
the individual bulk-micromachined wafer(s).
bonding time dependence of the fracture strength at
a certain temperature [6, 131. The authors suggest this
to be due to the elastic deformation of the contacting
wafers. The elasticity of the wafer increases with tem-
perature which would allow for extra bonds to form.
Silicon wafer-to-wafer bonding techniques can bas-
This theory is supported by an experiment that shows
ically be classified into two categories: fusion bonding
an increased fracture strength of thinned (and, there-
and intermediate bonding. Fusion bonding is based
fore, more elastic) wafers. The intrinsic void formation
solely on the direct adhesion of two wafers that are
is attributed to hydrocarbon contaminants at the wafer
brought into close contact at room temperature and
surface prior to the bonding and the annihilation of
subsequently heated up to about 1100 “C. Intermediate
their effect at temperatures beyond 800 “C .
bonding is based on the addition of a material in
between two wafers before pressing these together. This Beyond loo0 “C a maximum fracture strength of
intermediate can be a polymer glue, a low-temperature about 18 MPa is obtained with a void density that is
melting glass or a metal at eutectic temperature. The acceptable in most applications. Increasing the tem-
intermediate bonding usually requires a much lower perature beyond 800 “C is assumed to result in the
value of the processing temperature as compared to diffusion of oxygen into the crystal lattice and the
fusion bonding. replacement of oxide-bridge bonds by silicon-to-silicon
Silicon fusion bonding is based solely on the direct bonds in one of the theories [4, 11, 121. An alternative
bonding of two wafers that are brought into close theory assumes theviscous flow of oxide to be responsible
contact [I-4, 11, 121. No adhesion materials are added. for the increased fracture strength [3, 151. This viscous
The two wafers that are to be bonded have to be flat flow would also lead to the filling of microcavities at
(polished), clean and should be made hydrophilic the bonding interface that are due to the surface
(should contain a high density of OH groups attached roughness of the original wafers. The extrinsic void
to the surface) by boiling in nitric acid or immersion density is not reduced by this thermal treatment, so
in an H,O, N&OH bath. The wafers are brought into clean-room precautions have to be taken during bonding.
close contact at room temperature by either mechanical Notwithstanding the versatility and ease of operation,
 or electrostatic  means. The bonding is generally the silicon fusion bonding also shows two drawbacks.
The first major problem concerns the electrical inter- budget. The rapid thermal anneal is part of a two-step
connect between parts of the device located at different approach and is in principle very interesting, as it allows
wafers. A three-wafer capacitive accelerometer as shown an effective separation between the wafer-to-wafer align-
in Fig. 1 requires contacting to all wafer levels, whereas ment and pre-bond (at about 350 “C) and the high-
the mass wafer is the most suitable for the integration temperature rapid anneal for creating a reliable bond.
of the electronic circuits. The through-wafer intercon- This technique is compatible with smart sensors with
nect could be realized using a tapered multi-wafer stack respect to the negligible junction diffusion, however
and by placing wire bonds in between. The lateral the procedure is not compatible with aluminum on-
dimensions of the individual dies on the cap wafer wafer interconnect. The compatibility of the wafer-to-
should be smaller than those on the mass wafer and wafer bonding with integrated active devices in a stan-
the latter should be smaller than the die size of the dard process with the purpose of forming smart sensors
baseplate. The obvious disadvantage of this approach is, therefore, mainly limited by the on-wafer intercon-
is the increased Gomplexity of processing that is required nection problem.
to avoid loss of full wafer batch processing capability
(e.g. etching of V-grooves at the dicing lane in the cap
wafer and the mass wafer) and the increased costs of Low-temperature wafer-to-wafer bonding
bonding and packaging.
Secondly, the deposition of the on-wafer interconnect Intermediate bonding is the bonding of two silicon
and the subsequent patterning have to take place before wafers using an intermediate layer; a polymer glue, a
the wafer-to-wafer bonding. Therefore, the interconnect soft glass or gold beyond the eutectic temperature of
should be able to withstand the bonding temperature. the Au-Si binary system. The glue bonding is basically
The conventional material used for interconnect is simple; a thin and reasonably uniform layer can be
aluminum, which has a eutectic temperature at 577 “C. attached to the surface using spinning techniques. Press-
This implies that the aluminum becomes liquid at this ing the wafers together and subsequent curing results
temperature, which is due to the fact that it is contained in a bond. However, the glue bond is usually of poor
in the binary Al-Si composition, and consequently the reproducibility due to the limited control of the process.
pattern information is lost. The problem can in principle Corrosion due to outgassed products, thermal instability
be solved when resorting to s&ides. A number of and penetration of moisture limits the reliability .
micromechanical techniques are feasible to resolve the Moreover, the glue adhesion reveals only a limited
through-wafer interconnection problem. However, the compatibility with silicon processing. Nevertheless, this
key issue that limits the practical applicability of those technique has been successfully applied for the fab-
solutions is usually set by the processing temperature rication of SO1 devices .
and its influence on junction diision and the on-wafer Glass with a low softening temperature can be de-
interconnect. posited on a silicon wafer to serve as an intermediate
Conventional dopants in silicon (B, P and As) only bonding material . The temperature lowering is
demonstrate an appreciable diffusion at temperatures basically due to the addition of another substance. The
beyond 800 “C. Moreover, a rapid thermal anneal for resulting composition shows a phase diagram with a
3 min at 1100 “C has been reported to be sufficient eutectic temperature that is significantly lower than
for reliable wafer-to-wafer fusion bonding . This that of pure glass.
process step does not add significantly to the thermal One paper reports on the performance of #7570
glass . This is basically a lead borate glass with a
softening point at 440 “C. The bonding takes place
using both mechanical and electrostatic contact force.
A fracture strength in excess of 1.5 MPa is reported
for bonding at room temperature, a mechanical stress
of 100 kPa and an applied voltage in excess of 50 V.
/ \SEISMIC/ \ Although the authors do not provide much detailed
information about the nature of the bonding process
and the bonding mechanism at room temperature,
bonding is assumed to take place due to local heating
at the interface that results from the electrical current
Another report describes the silicon wafer-to-wafer
Fig. 1. Accelerometer with differential sense and servo drive bonding using boron-doped glass as the intermediate
capacitance. material . The glass is deposited on one of the
silicon wafers and subsequently this wafer is bonded Finally, there is the gold-silicon hard solder that has
to a second wafer at 450 “C. Bonding has been achieved, already been frequently used in VLSI for silicon die
however this technique is very sensitive to phosphorus bonding to a substrate . The silicon-gold binary
contaminants in the glass. Phosphorus leads to a drastic system reveals the most dramatic reduction of the
increase in the bonding temperature. melting temperature. As shown in Fig. 2, the melting
The performance of a bond based on sputtered #7740 temperature is reduced from 1063 “C at pure gold to
borosilicate glass has been reported [20, 211. A 1-5 363 “C!, whereby 19 at.% silicon is dissolved in the
pm thick layer is deposited on both wafers to be bonded. eutectic silicon-gold compound. Eutectic die bonding
The wafers are subsequently electrostatically bonded is often used in industry. An Au/Si compound with 19
at 400 “C with 50-200 V applied. The bonding takes at.% Si is used as a substrate and heated up to a
about 10 min. A typical fracture strength of 2.5 MPa temperature slightly above the eutectic temperature
was obtained. The bonding mechanism is generally (dashed line in Fig. 2). This Au/Si substrate acts as a
believed to be based on the drift of mobile sodium solder and consumes silicon from the die after it is
ions in the glass layers through the bonding interface, brought into direct contact. Silicon is dissolved until
although the same effect has been observed for sodium- the saturation composition is reached (X, in the Figure).
free glass . The glass, although an electrical isolator Upon cooling a reliable bond was obtained. An extension
at room temperature, is slightly conductive at the bond- of this technique is the micron bump bonding, in which
ing temperature. The material is depleted near the multi-electrode contacts can be made between a die
interface due to the electrostatic repelling of ions. The and the SilAu substrate. Although this technique has
voltage drop is, therefore, localized near the interface so far only been used in die bonding, it can in principle
and a sufficient electrostatic contact force is available. also be employed for silicon wafer-to-wafer bonding
Recently, wafer-to-wafer bonding has been reported with gold as an intermediate layer.
using sodium silicate as an intermediate layer . A Eutectic gold bonding has already been implemented
diluted solution of sodium silicate in water is spun onto in 1979 by Ko et al.  for the fabrication of pressure
one of the wafers to be bonded and after bringing the transducers. This type of bond seems to introduce
wafers into contact at room temperature and a sub- problems in the long-term stability of the sensor. The
sequent anneal at 200 “C for 2 h, a bond with a surface thermal mismatch introduces stress during cool down
energy of 3 J/m’ was obtained. This value is comparable that relaxes with time. These problems will be dem-
with the bonding strength for conventional silicon-to- onstrated to be basically due to an insufficient tem-
silicon bonding at an anneal temperature in excess of perature control during bonding.
1000°C, mentioned in the previous section. The obvious
disadvantage of this technique is the introduction of
Weight % Si
sodium at the interface. However, the effect of the Au 2 4 6 8 10 15 20 2530 40 60 Si
mobile oxide charge on the performance and reliability I 1 , I I I I I I 1 I III8
of integrated active devices is likely to be very limited, I I I I I I I t I
due to the fact that the bonding is performed as a
post-processing step at low temperature. 1412
Wafer-to-wafer bonding has also been demonstrated
using metallic intermediate layers. Ti , PtSi [W]
and TiSi,  have been reported to give reliable
bonding after an anneal at 700 “C. In the case of
titanium, a 5000 A layer is E-beam evaporated on both
wafers to be bonded. Subsequently, the wafers are
brought into contact at room temperature and annealed
at 700 “C in an oxidizing ambient for 20 min. The
operating mechanism is believed to be similar to the
silicon-to-silicon direct bonding, viz. via the formation
of Ti-O-Ti bridges. Platinum silicides can be formed
by E-beam evaporation of Pt while keeping the substrate
at 350 “C. After etching of the Pt layer on top of the
formed PtSi, the two wafers to be bonded are brought
into contact at room temperature and annealed in a
nitrogen ambient for 2 h at 700 ‘C. The special property Au 10 20 30 40 50 60 70 80 90
Atom % Si
of the silicide-based bond is the good electrical contact
between the two bonded wafers. Fig. 2. Silicon-gold phase diagram.
Si/Au wafer-to-wafer bonding suggests that the mixing of Si into Au due to solid-
state diffusion does not take place uniformly until the
Eutectic gold die bonding is basically the de facto eutectic composition is reached (19 at.% Si), but rather
industry standard on die bonding and the application clusters of silicon are formed. Obviously, reliable bond-
in silicon wafer-to-wafer bonding seems like an obvious ing cannot be achieved after microstructure formation,
extension. Problems associated with gold eutectic bond- as only point-to-point contact is made where ridges
ing are the long-term drift in sealed-cavity devices and overlap.
the possible trap formation halfway to the bandgap. Bonding strength was evaluated using both the razor
Contamination of silicon with gold would result in a blade insertion test (razor should not penetrate) and
severe reduction of the minority carrier lifetime in by SEM observation of the cleaved bonded wafers [6,
integrated active devices. However, many microma- 241. Figure 4(a) and (b) shows the detailed and wide
chining processes are already designed in such a way view, respectively, and indicates a bonded area less
that the actual micromachining steps are performed as than 50% for bonding at 400 “C almost irrespective of
low-temperature post-processing steps outside the clean- bonding time. Experiments indicate that a reliable bond
room. The intermediate eutectic gold bonding would with in excess of 90% bonded area is obtainable for
be a natural extension of this approach. Under normal bonding at 365 “C and 10 min, as shown in Fig. 5.
conditions silicon dissolves in the flowing gold and not Bonding time and temperature are very critical, however
vice versa, so there is, in principle, no gold doping of the texture of a monitor wafer can be used as a simple
Standard 3” p-type (100) Si wafers were thermally
oxidized and 300 A Ti and 1200 8, Au were subsequently
E-beam evaporated. The Ti is deposited to avoid poor
adhesion due to the low-surface energy SiO, layer.
Finally, the wafers are brought into contact and placed
on a hot plate with a 100 g distributed weight for
between 5 and 4000 min at temperatures between 350
and 400 “C!. Heating of the wafer beyond the eutectic
temperature results in a change in surface texture due
to the formation of fine silicon microstructures on top
of the gold surface as shown in Fig. 3. This effect is
already known from die bonding  and indicates
that a 100% bonded area cannot be achieved. Although
the shape and density of the final microstructures is
almost time and temperature independent, the effect
occurs after 60 s at 400 “C, 100 s at 390 “C, 5 min at
370 “C and 10 min at 365 “C. This observation strongly (4
Fig. 3. Structure of the Au/Si eutectic material after beating up Fig. 4. Detailed (a) and global (b) view of the eutectic bond
to 390 “C. after bonding at 400 “C for 4000 min.
on eutectic silicon-gold intermediate bonding. Smart
micromechanical sensors and actuators can be fabricated
with electronic and/or micromechanical functions dis-
tributed over various wafers, due to the low-temperature
processing and the implementation of through-wafer
interconnect. The area consumption required for bond-
ing (sealing) and etching of through holes makes the
technique less-suitable for high-density wafer-scale in-
tegration, but it is of great promise in smart sensors,
where up to 10 leads is usually sufficient.
This work is supported in part by STW Project No.
Fig. 5. The eutectic bond after bonding at 365 “C for 10 min.
indicator. Experiments have demonstrated the suitability
of the eutectic low-temperature wafer-to-wafer bonding References
for multi-wafer smart sepsors, the compatibility with
techniques for through-wafer interconnect and the func-
1 H. Ohashi, K. Furukawa, M. Atsuta, N. Nakagawa and K
tional integrity of the bonded device. The sealing per- Imamura, Study of %-wafer directly bonded interface effect
formance needs to be demonstrated using an endurance on power device characteristics, Proc. IEDM ‘87, pp. 678-681.
test on an integrated pressure sensor. 2 J.B. La&y, S.R. Stiffler, F.R. White and J.R. Abernathy, SOI
This technique is compatible with on-wafer aluminum by bonding and etch-back, Proc. IEDM ‘85, pp. 684-688.
3 W.P. Maszara, Silicon-on-insulator bywafer bonding: A review,
interconnect. The Si/Al binary system has a eutectic J. Elechwc~em Sac., 138 (1991) 341-347.
temperature at 577 “C and is, therefore, not flowing 4 M. Shimbo, K. Furukuwa, F. Fukuda and K. Tanazawa,
at %/Au eutectic bonding. The aluminum on-wafer Silicon-to-silicon direct bonding method, 1. Appl. Phys., 60
interconnect can be deposited and patterned before (1986) 2897-2989.
the wafer-to-wafer bonding. In reality the problems are 5 T.R. Anthony, Dielectric isolation of silicon by anodic bonding,
.J. Appl. Phys., 58 (1985) 1240-1247.
more complicated. First, the bonding temperature of
6 W.P. Maszara, G. Goetz, A. Caviglia and J.B. McKitterick,
400 “C has the same effect on the patterned aluminum Bonding of silicon wafers for silicon-on-insulator, J. Appl.
on one of the silicon wafers as sintering and care should Phys., 64 (1988) 4943-4950.
be taken to avoid spiking. On the other hand it should 7 L.J. Spangler and K.D. Wise, A bulk silicon SOI process for
be possible to combine the bonding and sintering. active integrated sensors, Sensors and Actuatm, A24 (1990)
Secondly, the silicon dissolves to,some extent into the
8 R.W. Bowen, MS. Ismail and S.M. Farrens, Aligned wafer
aluminum . Finally, stress is formed or relieved in bonding: a key to 3-dimensional microstructures, J. Electron.
the interconnect at this temperature by elastic or plastic Mater., 20 (1991) 383-387.
deformation  and the reliability of the device could 9 K.P. Petersen, P. Barth, J. Poydock, J. Brown, J. Mallon and
be severely impaired by the resulting voids . These J. Bryzek, Silicon fusion bonding for pressure sensors, Proc.
1988 Solid-State Sensors and Actuate Workshop,H&on Head
problems have not yet been fully investigated. Island, SC, USA, June 6-9, 1988, pp. 144-147.
The next issue is the through-wafer interconnect, 10 P. Barth, F. Pourahmadi, R. Mayer, J. Poydock and K.P.
which can be based on optical techniques , aluminum Petersen, A monolithic accelerometer with integral air damp
electromigration  or bulk micromachining . The ing and overrange protection, I+vc. 1988 Solid-State Sensors
bulk micromachining of pits through a wafer and a and Actuators Workshop, Hilton Head Island, SC, USA, June
6-9, 1988, pp. 35-39.
subsequent metal coating of the bevels is presently 11 P.W. Barth, Fusion bonding for fabrication of sensors, ac-
being investigated, as is its compatibility with gold tuators and microstructures, Sensors and Actuarors, A21-A23
intermediate bonding . (1990) 919-926.
12 C. Harendt, H-G. Graf, B. Hoemnger and E. Penteker,
Silicon fusion bonding and its characterization, J. Micromech.
Mictveng., 2 (1992) 113-116.
13 Q.-Y. Tong, X.-L, Xu and H. Shen, Diffusion and oxide
viscous flow mechanism in silicon direct bonding process and
A low-temperature process has been designed for silicon wafer rapid thermal bonding, Electron. Lett., 26 (1990)
the fabrication of wafer-to-wafer bonded devices based 697-699.
14 K. Mitani, V. Lehmann and U. Gosele, Bubble formation 24 D. Noyak, A. Reisman and I. Turlik, Metal-to-metal bonding
during silicon wafer bonding: Causes and remedies, Pmt. using an oxidizing ambient atmosphere, J. Ekxtochem. Sot.,
1990 Solid-State Sensors and Actuators Worhshop, Hilton Head 135 (1988) 1023-1025.
2.5 M.S. Ismail and R.W. Bower, Platinum silicide fusion bonding,
Islanrl, SC, USA.
Elecnon Len., 27 (1991) 11X3-1155.
1.5 R. Stengl, T. Tan and U. Gosele, A model for the silicon
26 M.S. Ismail, R.W. Bower and B.E. Roberds, Polysilicon and
wafer bonding process, I. Apple Phys., 28 (1988) 17351741.
Jpn. titanium silicide+polycide fusion bonding for 3-D micro-
16 R.K. Shukla and N.P. Mencinger, A critical review of VLSI devices aoolications. Pmt. 1992 Solid-State Sensors and Ac-
die-attachment in high-reliability applications, SolidState Tech- taators W&shop, kton Head Island, SC, USA, pp. 86-89.
no!., (July) (1985) 67-74. 27 W.H. Ko, J. Hvnecek and S.F. Boettcher. Develooment of
17 T. Hamaguchi, N. Endo, M. Kimura and M. Nakamae, Novel a miniature pressure transducer for biomedical applications,
LSI/SOI wafer fabrication using device layer transfer tech- IEEE Trans. Electron Devices, ED-26 (1979) 18961905.
28 G.J. van Gurp, Diffusion-limited silicon precipitation in evap-
nique, From. IEDM ‘86, pp. 688-691.
orated AvSi films, J. Apple Phys., 44 (1973) 2040-2050.
18 M. Esashi, N. Nakano, S. Shoji and H. Hebiguchi, Low- 29 D.S. Gardner and P.A. Flmn, Mechanical stress as a function
temperature silicon-to-silicon anodic bonding with interme- of temperature in aluminum films, IEEE Trans. Electron
diate low melting point glass, Sensors and Actuators, A21-A23 Devices, ED-35 (1988) 2160-2169.
(1990) 931-934. 30 KHinode, I. Asano and Y. Homma, Void formation mech-
19 LA. Field and R.S. Muller, Fusing silicon wafers with low anism in VLSI aluminum metaliiation, IEEE Trans. Electron
melting temperature glass, Sensors and Actuators, A2Z-A23 Devices, ED-36 (1989) 1050-1055.
31 LA. Homakand SK. Tewksbury, On the feasibility of through-
wafer optical interconnects for hybrid wafer-scale integrated
20 A.D. Brooks, R.P. Donovan and C.A. Hardesty, Low-tem- architectures, IEEE Trans. Electron Devices, ED-34 (1987)
perature electrostatic silicon-tosilicon seals using sputtered 1557-1563.
borosilicate glass, .7. Electrochem Sot., II9 (1972) 545-546. 32 H.E. Cline and T.R. Anthony, Migration of fine molten wires
21 A. Hanneborg, Silicon-to-thin film anodic bonding, J. Micro- in thin silicon wafers, J. Appl. Phys., 49 (1978) 2412-2419.
mech. Microeng., (1992) 117-121. 33 J.C.-M. Huang and K.D. Wise, A monolithic pressure-pH
22 R.C. Frye, J.E. Griffith and Y.H. Wong, A field-assisted sensor for esoohaaeal studies. Proc. IEDM ‘82. San Francisco.
CA, USA, LkG. I& 1982;pp. 316-319.
bonding process for silicon dielectric isolation, 1. Elechochem.
34 R.F. Wolffenbuttel and K.D. Wise, Bulk-micromachined
Sot., 133 (1986) 1673-1677. through-wafer interconnect for silicon wafer-to-wafer bonding,
23 H.J. Quenzer and W. Beneke, Low-temperature silicon wafer Proc. Tmnsducer ‘93, Yokohama, Japan, June 7-10, 1993, pp.
bonding, Sensor and Actuators A, 32 (1992) 340-344. 194-197.